Memoria de Trabajos de Difusin Cientfica y Tcnica, nm. 10 (2012) 45
ISSN 1510-7450 ISSN (en lnea) 1688-9584
Superplasticity of ultrafine grained low-alloy steels
Superplasticidad de aceros de baja aleacin con grano ultrafino
Sara Fernandez1, Mara Jos Quintana2, Jos Ovidio Garca1, Luis Felipe Verdeja1, Roberto
Gonzlez2, Jos Ignacio Verdeja1
Recibido: Agosto 2012 Aprobado: Setiembre 2012
Resumen.- Los aceros con estructura de grano ultrafino pueden presentar comportamiento superplstico a temperaturas y velocidades de deformacin especficas, que faciliten la activacin de los mecanismos de deslizamiento de fronteras de grano. El comportamiento superplstico implica deformaciones elevadas por procesos de deslizamiento de fronteras de grano con acomodo de materia por difusin, tal como lo describe el modelo de Ashby-Verrall. El trabajo presenta pruebas de tensin a temperatura elevada en aceros de bajo carbono y baja aleacin obtenidos por procesos avanzados de rolado controlados termomecnicamente, mostrando a 800C elongaciones de hasta el 200%. La microestructura del acero se analiz para poder identificar las fronteras de grano de la ferrita y de la perlita, y su interaccin despus de que la probeta fue deformada. Las tcnicas de microanlisis (ptico y SEM) muestran evidencia de: crecimiento de defectos que impiden alcanzar elongaciones a ruptura mayores, flujo no uniforme (movimiento-rotacin relativo de granos prximos entre s) y deformacin intergranular no-superplstica (flujo cuasi-uniforme), resultando todo esto en fractura prematura.
Palabras clave: superplasticidad, grano ultrafino, coeficiente m de velocidad de deformacin, deslizamiento de fronteras, aceros de alta resistencia y baja aleacin.
Summary.- Write Steels with ultrafine grained structure may present superplastic behavior at specific temperatures and strain rates that allow the grain boundary sliding mechanisms to be activated. The superplastic behavior implies deformation to large strains by grain-boundary sliding with diffusional accommodation, as described by the Ashby-Verrall model. The work presents high temperature tension tests in a low carbon, low alloy steel obtained by advanced thermomechanical controlled rolling processes, showing at 800C elongations as high as 200%. The microstructure of the steel was analyzed in order to identify ferrite and pearlite grain boundaries, and their interaction after the specimens were deformed. Microanalytical techniques (Optical and SEM) show evidence of: damage growth that prevents the development of higher elongations to failure, non-uniform flow (relative movement-rotation of grains in close proximity to each other) and intergranular non-superplastic deformation (quasi-uniform flow); thus leading to premature failure.
Keywords: superplasticity, ultrafine grained, strain rate m coefficient, boundary sliding, high-strength low alloy steels (HSLA steels)
1. Introduction.- Superplasticity is the ability of polycrystalline solids (metals) to achieve extremely high and uniform elongations (from 100 to 1000%) when applying tensile stresses. The high dependency between the creep tension stress and the strain rate results in the lack of necking (or a series of diffuse necks) along the test zone of a specimen . From a
1 E.T.S.I.M.O., Universidad de Oviedo, Independencia 13, Oviedo 33004, Spain, Tel. (34) 985 10-43-03, Fax. (34) 985 10-42-42, [email protected] 2 School of Engineering, Universidad Panamericana, Augusto Rodin 498, 03920, Mxico, D.F., Mexico, Tel. (52)55 1251-6859, Fax. (52)55 5482-1600 ext. 6101, [email protected]
Superplasticity of ultrafine grained low-alloy steels S. Fernndez y otros
46 Memoria de Trabajos de Difusin Cientfica y Tcnica, nm. 10 (2012)
ISSN 1510-7450 ISSN (en lnea) 1688-9584
microstructural point of view, superplasticity is achieved when two mechanisms take place in the material: grain boundary migration and grain boundary shearing/sliding. Theoretical and microstructural models agree that the most important feature of this behavior is the grain boundary sliding (GBS). Nevertheless, dislocations or diffusion in grains or in zones near grain boundaries are necessary in order to maintain the superplasticity of the material .
Four essential characteristics  are required in a material for it to be considered superplastic: a stable microstructure of fine equiaxed grains , coefficient (strain-rate sensitivity exponent; ) values between 0.3 and 0.7, slow strain rates (10-3 to 10-5 s-1) and grain boundaries of the material that allow grain sliding and rotation when stress is applied .
In addition to the previous requirements, it is necessary to deform the material at the right temperature which is a fundamental characteristic in some superplastic behavior models, such as the one established by Ashby and Verrall . Their model proposes a theory (Grain Boundary Sliding, Diffusion Accommodated Flow Rate Controlling) to describe superplasticity taking into account two mechanisms: (a) the diffusion-accommodated flow (D-A flow), consisting of GBS along with material transport through grain boundary and bulk crystal diffusion  to maintain grain continuity (this phenomena dominates in the low stress regime, strain rates less than 10-5 s-1) and (b) the ordinary power-low creep (dislocation creep) which is a quasi-uniform flow mechanism that results in grain-elongation as dislocations accumulate as cells, storing energy; this last mechanism dominates at sufficient high stresses (strain rates higher than 10-3 s-1). In the intermediate stress range, both mechanisms compete in order to achieve the superplastic behavior.
The work presents the high temperature superplastic behavior of an UFG steel microalloyed with Ti-Nb obtained by Advanced Thermomechanical Control Rolling Processes (ATMCRP) at the Arcelor Mittal factory in Veria (Gijn, Spain), as materials of this type can show this behavior when certain conditions are met. The characteristics of the steel, delivered in the form of 27.6 mm in thickness sheets (around one inch), are described in the experimental procedure. The HSLA steels described in Euronorms 10149-2 and 10051 are examples of these materials, as well as other construction steels or automotive special steels (just as the ones described in the ultralight steel auto body ULSAB project), resulting in lower cost materials and a step forward in the research for better materials in industry, such as lightweight structures and components with very good weldability and easier to recycle, all of this, reducing the cost of the alloy and meeting high specifications with steels that have a lower amount of alloying elements and that are considered high-tech . Furthermore, ultrafine grained steels (UFG) may be applied in the future in most of the steel markets and can be used in other industrial applications, such as the ones that require superplastic behavior, just as this work demonstrates.
Ultrafine grained steels (grain size d 15m) are currently intensively studied worldwide, as they offer a solution to finding very high strength materials. They also present high toughness and are produced from standard steel compositions (which reflects in low cost) . Recent works have shown that the ultrafine grained structure may be obtained in a hot rolling mill by ATMCRP and not only from small scale laboratory tests [4,10]. However, under some circumstances these materials may present an important disadvantage as they exhibit unstable plasticity upon yielding, severely restricting its potential uses . In order to avoid this instability  the mechanical behavior of the steel must show a strain hardening coefficient n (as measured by tension test with the ASTM standard) higher than 0.1, in its hot rolling raw state. If this is achieved, the steel can be used for cold-work operations such as bending, stretching and drawing and in commercial applications such as automotive and other manufacturing industries .
A large number of non-ferrous alloys show superplasticity behavior during isothermal tensile testing. This behavior is characterized by large elongations, usually higher than 100% and sometimes reaching 1000% or more. Superplasticity, object of numerous research activities that started in the 19601970s, has the following properties:
S. Fernndez y otros Superplasticity of ultrafine grained low-alloy steels
Memoria de Trabajos de Difusin Cientfica y Tcnica, nm. 10 (2012) 47 ISSN 1510-7450 ISSN (en lnea) 1688-9584
high strain rate sensitivity to the flow stress as the essential and unique characteristic of superplasticity ,
strong variation of properties as a function of grain size and strain rate , relevance of grain boundary sliding in the deformation mechanism , vacuum forming of the metal sheet when deformed against the die  and grain boundary sliding by diffusion and accommodation processes . In other words, in order for the superplastic behavior to show high strain rate sensitivity, high temperature testing (> Tm), a fine microstructure and a relatively low strain rate are required [16-18].
2. Experimental procedure and Results.- The specified chemical composition for this steel (in weight %) according to the Euronorm is: C 0.168, Mn 1.361, Si 0.453, P 0.022, S 0.009, Cu 0.026, As 0.003, Al 0.028, Cr 0.035, Ti 0.026, V 0.002, Nb 0.033, Mo 0.004, Ni 0.031, Sn 0.002, Al (soluble) 0.027, B 0.0001, N 0.0055, Zr 0.0000, C